Int. J. Electrochem. Sci., 13 (2018) 11691 – 11701, doi: 10.20964/2018.12.13
International Journal of
Effects of Particle Conductivity on the Fe-Si co-deposition
Qiong Long1,2*, Yunbo Zhong2, Yujiao Wu1, Yingzhe Zhang1
1 Guizhou Key Laboratory for preparation of light metal materials, Guizhou Institute of Technology Guiyang 550003, China
2 State Key Laboratory of Advanced Special Steel, College of Materials Science and Engineering, Shanghai University, Shanghai 200072, PR China
Received: 14 August 2018 / Accepted: 23 September 2018 / Published: 5 November 2018
Composite iron deposits containing non-conductivite Si particles and conductive Si-Fe alloy particles with an average size of 1μm were prepared in circulating solution, the effects of particle conductivity on the co-deposition process of particles were investigated. The results show that high conductivity contributed to the co-deposition process of particles into the composite coatings, and in a mode of "cladding" for the co-deposition of conductive Si-Fe particles, while that for non-conductive Si particles was "embedding" mode. At the same time, with increasing the conductivity, the co-deposition process of particles was obviously deviate from the Guglielmi model. A possible mechanism on the forming process was discussed.
Keywords: Fe-Si coating; Electrodeposition;Particle; Conductivity; Co-deposition
As a high efficient and green technology, composite electrodeposition has many advantages such as low temperature, low cost and little environmental pollution. In recent years, composite electrodeposition technology has been developing rapidly and widely applied in aerospace, transportation, repair, functional material and decoration etc.[8-12]. The content and distribution of inert particles in the coating often become the key factors affecting the composite coating[13-15]. Pan proposed to prepare 6.5wt%Si silicon steel strip by composite electrodeposition with Si-Fe alloy particles or pure Si particle, and found that the silicon content of coatings can reach 6.45%, while that only 3.45% when applied pure silicon particles. Long also found that increasing the silicon content of iron-silicon particles with an average size of 2.5μm, the co-deposition process of particles was more difficult, and it can be attributed the conductivity of the particles decreased significantly, but the adsorption mechanism needs for further study. So far, electrodeposition containing particles in the composite coatings were main ceramic and nano-scale particle[18-19], there are few research to prepare composite coating with micro-scale and conductive particles.
Therefore, the Fe-Si coating with different conductive Si-Fe alloy particles and pure Si particles was prepared in this paper, and the influence of particle conductivity on the co-deposition process was investigated, and the possible mechanism of the effects was discussed in detail.
Pure Si particles and Si-Fe powders with mass fraction of 30%, 50% and 70% were used to prepare composite coatings. Figure 1 gives the distribution range of particle diameter tested by particle diameter sizer(Mastersizer 2000). From Figure1, it can be found that the average particle diameter was about 1μm, and the distributions were similar for these different types of particles. The basic plating solution was 250g/L FeSO4·7H2O, 50g/L FeCl2·4H2O, 50g/L NH4Cl, all the chemicals were analytical grade and the distilled water was used for preparing all kinds of solution. Meanwhile, using the hexadecyl trimethyl-ammonium bromide(HTAB) with the concentration of 0.2g/L as the dispersing agent to prevent the adopted particles from agglomeration in the plating bath.
0.0 0.5 1.0 1.5 2.0
2 4 6 8 10 12 14
Fe-30wt% Si powder Fe-50wt% Si powder Fe-70wt% Si powder Si powder
Figure 1. distributions of particles diameter
value to1.5 with dilute H2SO4(0.5mol/L), and the electroplating solution was agitated with high purity argon bubbles to reduce the oxygen content in the solution. In the electrodepostion process, circulating plating solution to prevent the settlement of particles. At the same time, electroplating solution was introduced into electrolytic bath using inverted funnel, and a couple of grid baffle with round holes of 3 mm diameter was installed at 10 mm in front of electrodes to avoid the scouring action of electrolyte on the electrode surface(Figure 2). The plating process was maintained at 298 K and the plating time was 30min, and the surface morphologies, cross-sections and analyzing the concentration of silicon in the composite coatings were characterized by scanning electron microscopy(SEM) with energy dispersive X-ray spectrometer(EDS) and checking the distribution of particles. The conductivity of Fe-Si alloy powder was estimated by Fe-Fe-Si alloy bar with diameter of 8mm and length of 10mm. First of all, iron powder and silicon powder were mixed uniformly in the proportion of 30wt%, 50wt% and 70wt%, and added in the induction furnace with high vacuum and high purity argon shielding gas respectively. After fully melting, the Fe-Si alloy ingots were casted into a bar with quartz tube by suction casting, and then the resistance(R) of the alloy bars was measured by a four-probe resistivity measurement setup composed of a Keith-ley 2400 digital source meter and a Keithley 2182A nanovoltmeter(America). The conductivity of the Fe-Si alloy bars was calculated via L/RS, L and S in the formula were the length of alloy bar and the area of cross-section, respectively. The element distribution in the alloy bars obtained by suction casting was uniform, so the conductivity of the alloy bars can be used to characterize the conductivity of the particles.
Figure 2. Schematic diagram of the experiment equipment
3. RESULTS AND DISCUSSION
9.76wt% for 30wt%Si-Fe particle at the 50g/L of particle concentration and 2A/dm2 current density, whereas that for Si particles was only 4.48wt%. However, after the particle concentration was more than 50g/L, the silicon content of coatings increased relatively stable. Simultaneously, as the increase of the current density, the silicon content of coatings increased and reaching a maximum value at 2A/dm2, and then decreased as current density continuing increasing.
Figure 3. SEM micrographs of Fe-Si coatings for 30wt%Si-Fe powder(a), 50wt%Si-Fe powder(b),
70wt%Si-Fe powder(c) and pure Si powder(d) at 2 A·dm-2 with the particle concentration of 50 g·L-1
Figure 4. Cross-section morphologies of Fe-Si coatings at 2 A·dm-2 (a)30wt%Si-Fe powder (b)
50wt%Si-Fe powder (c)70wt%Si-Fe powder (d) Si powder
0 30 60 90 120 150 2
4 6 8 10 12
Particle concentration, g/L
0 20 40 60 80 100 120 140 160 2
4 6 8 10
Particle concentration, g/L
0 20 40 60 80 100 120 140 160 2
4 6 8 10
Particle concentration, g/L
0 20 40 60 80 100 120 140 160 0
1 2 3 4 5 6 7 8
Particle concentration, g/L
Figure 5. Silicon content of coatings under different particle concentrations and current densities for
(a) 30wt%Si-Fe powder; (b) 50wt%Si-Fe powder; (c) 70wt%Si-Fe powder; (d) Si powder
Relatively larger particles with about 2.5 μm diameter were used to prepare Fe-Si composite coatings in our previous work. To ensure that particles are uniformly suspended in solution by means of downward mechanical stirring owing to the great gravity effect. However, a strong scouring effect will be induced by the strong stirring effect on the electrode surface, which was undesirable to the adsorption process of particles into the composite coating. Under the optimum electroplating condition, approximately 6wt% silicon content of coatings can be obtained for the 30%Si-Fe powder with the particle concentration of 50g/L, whereas for Si powder was only about 2wt%. Therefore, in order to reduce these adverse effects, the small-size particles with the 1 μm of average particle size were used to prepare Fe-Si coating in this paper, and the final settling velocity of particles in the electroplating solution is relatively small according to the Stokes Formula, which will be addressed later. At the same time, cycle stirring solution in a downward direction, inverted funnel and a pair of baffles above the electrodes were applied(Figure 2), which can further reduce the scour effect of solution flow on the electrode surface. As a result, it should be helpful for the adsorption process of particle, and the co-deposition process of particles entering the Fe-Si composite coating was investigated.
According to Guglielmi N, the particle inclusion in metal matrix from electroplating solution occurs in two consecutive steps of adsorption, including the "loose adsorption" and "strong adsorption". The inert particle on its way from the bulk of the solution to the site of incorporation at the active cathode surface will proceed through the flowing stages(Figure 6): Firstly, particle surface adsorbs some cations and moves towards the hydrodynamic boundary layer(δ0) by forced
cathode surface is uniformly accessible for the inert particles and the plating solution.
Figure 6. The stages in the co-deposition of a particle
The Guglielmi model may be expressed as follows：
) 1 ( )
( ( )
c k e
nF Mi a
Where cv and av are the volume fraction and volume fraction of the particle in the electroplating
solution and composite coatings respectively, F is the Faraday constant, the ρm, M and n are the
density, atomic weight and the valence of electro-deposited metal respectively, η is the cathodic overpotential, A is the constant in the kinetic equation of electrochemical reaction A
i 0 , i0 is the
exchange current density, k is the Langmuir isotherm constant, B and υ0 are the constants related to the
co-deposition process of particle. From the equation(1), when current density at the same value, (1-av)cv/av has a linear relationship with cv, and the slope of each line can be expressed as follows:
tan A B
When (1-av)cv/av equal to 0, the intercept of each line can be calculated and therefore the value
also can be derived. Figure 7 gives the relationship between (1-av)cv/av and cv at different
current density and particle concentration for Si and 70wt%Si-Fe particles. It can be found that the (1-av)cv/av was linear with the cv for the Si particle. When the current density is less than 2A/dm2, the
slope of the fitting straight line for (1-av)cv/av and cv under different current density will extend to the
A0 on the X axis(Figure 7a), indicating that the adsorption of particles basically obeys Guglielmi model. When the current density was higher than 2.5A/dm2, the intersection on the X axis deviates from the A0, so the adsorption process of the particles deviates from the Guglielmi model, which was not consistent with Celis and Suzuki’s similar research[22-23]. When using 70wt%Si-Fe particles, although showed a linear relationship between (1-av)cv/av and cv in the current density of no more than
relationship, especially when the concentration of plating particles was less than 0.01(Figure 8). Therefore, the co-deposition process for 30wt%Si-Fe and 50wt%Si-Fe particles obviously disobeyed the Guglielmi's model under different current density.
-0.030 -0.015 0.000 0.015 0.030 0.045 0.060
0.1 0.2 0.3 0.4 0.5 0.6 (a) A0 0.5A/dm2 1A/dm2 1.5A/dm2 2A/dm2 2.5A/dm2 3A/dm2 4A/dm2 （ 1-a v )cv /av cv
-0.02 -0.01 0.00 0.01 0.02 0.03 0.04 0.05
0.00 0.05 0.10 0.15 0.20 0.25 0.30 (b) 0.5A/dm2 1A/dm2 1.5A/dm2 2A/dm2 2.5A/dm2 3A/dm2 4A/dm2 B0 （ 1-a v )cv /av cv
Figure 7. The relationship between (1-av)cv/av and cv of (a) pure Si and (b) 70wt%Si-Fe powders
-0.005 0.000 0.005 0.010 0.015 0.020 0.025
0.01 0.02 0.03 0.04 0.05 0.06 0.07 0.08 0.09 0.005 0.010 0.01 0.02 0.03 0.04 (a) 0.5A/dm2 1A/dm2 1.5A/dm2 2A/dm2 2.5A/dm2 3A/dm2 4A/dm2 (1-a v )cv /av cv
-0.007 0.000 0.007 0.014 0.021 0.028 0.035
0.03 0.06 0.09 0.12 0.15 0.18 0.21 0.005 0.010 0.02 0.04 0.06 0.08 0.10 (b) 0.5A/dm2 1A/dm2 1.5A/dm2 2A/dm2 2.5A/dm2 3A/dm2 4A/dm2 (1-a v )cv /av cv
Figure 8. The relationship between (1-av)cv/av and cv of (a)30wt%Si-Fe and (b)50wt%Si-Fe powders
During the co-deposition process of particles on cathode surface, the reaction constant(κ) can be expressed as：
Where ka and kd respectively are the adsorption and desorption coefficient of particles on the
electrode surface. Thus, if k＞1, it can be deduced that the adsorption rate of particles is faster than the desorption rate. The Guglielmi’s model implies the Langmuir adsorption isotherm can be modified simultaneously as follows:
(1- ) + 1 = θ kc kc σ υ
plating solution with 30wt%Si-Fe powder was only 30wt% of the Si powder when the concentration of particles in electrolyte at the same value, which further indicated that the co-deposition of 30wt%Si-Fe particles were more easily compared with Si particles. Thus, it is essential to discuss the effects of properties of applied particles on the co-deposition process.
During the composite electro-deposition process, the final settling velocity of particles in the electroplating solution by Stokes formula can be given as follows：
18 ) (
Where υ is the settling velocity, d is the diameter of particles, ρs and ρ is the density of particle
and electrolyte solution, g is the acceleration of gravity; and μ is solution viscosity. According to formula(5), it indicates that a greater density of particles will lead to the greater final settling velocity of particles, which is not conducive to being captured by the reduced metal ion. The effects of silicon content on the particle density and ration of final settling velocity were showed in Figure 9. However, above results show that the Si-Fe particles are easier to enter the coatings then Si particles, which indicates that the density of the particles is not the key factor affecting the co-deposition process of particles.
20 30 40 50 60 70 80 90 100 110 1000
2000 3000 4000 5000 6000 7000
1 2 3 4 5 6 7
The silicon content of particles, wt%
Figure 9. Effects of silicon content on the density and ration of final settling velocity of particles
the particle surface after the 30wt%Si-Fe particle contacted to the cathode surface, owing to it was conducive to the co-deposition process of conductive 30wt%Si-Fe particles. In other words, the conductive Si-Fe particles into the composite coating in the mode of "cladding", and the Si particles with poor conductivity into the coating in "embedding" mode. Meanwhile, it is obvious that was in accordance with the surface morphologies and cross-sections of corresponding Fe-Si composite coatings(Figure 11).
Table 1. Conductivities of different types of particles and electrolyte
Particulate silicon content (wt%) 30 50 70 100
Conductivity（S·m-1） 4.79×105 2.63×105 6.52×103 2.52×10-4
Figure 10. Electrolytic current distributions in the vicinity o f applied particles and schematic views of
composite electrodeposition for nonconductive particles( a-b ) and conductive particles(c-d )
Figure 11. Surface morphologies and cross-sections of coatings for Si powder(a-b) and 30wt%Si-Fe
Further more, the current density also had a great influence on the co-deposition process of particles. Above results revealed the silicon content of coatings increased for all the different types of particles with increasing the current density, and reaching a maximum value at 2 A·dm-2, and then decreased if continuing to increase the current density. During the electro-deposition process, the particles adsorbed ions migrated to cathode surface from solution under the effects of different forces, including electric force, natural convection and gravitational force, and some of them could be captured by the growing metal, then entered the coatings completely. Therefore, it can be deduced that the transfer rate of particles was faster than the growth rate of iron metal when the current density is less than 2 A·dm-2, and reversed while above 2 A·dm-2. Meanwhile, the standard electrode potential of Fe2+ is -0.44V, the polarization would significantly increased with the increase of current density. Therefore, an intensive hydrogen evolution reaction will always accompany the electro-deposition process, which provide additional agitation in the cathode surface, and it can be expressed in formulas (7) and (8):
Fe2++2e-→Fe (6) H+ + e- → Had (7) Had + Had→H2↑ (8)
A proper agitation can strengthen mass transfer of solution and may boost the incorporation of particles. However, too strong agitation will significantly reduce the co-deposition of particles, owing to the particles can be taken away by the turbulent flow induced by hydrogen evolution from the cathode surface before being incorporated completely. The current efficiency in the process of iron plating is approximately 65%[26-27], which indicated that the reaction of hydrogen evolution was very strong. Too large electroplating fluid disturbance affect the adsorption process of particles, reducing the rate of particles entering the composite coating. Thus, when the current density exceeds 2.5A/dm2, the co-deposition process of Si particles was obviously deviated from the Guglielmi’s model.
The Fe-Si composite electrodeposion have been conducted in the condition of circulating electroplating solution at a temperature of 298 K in a sulfate-chloride plating bath. The effects of particle conductivity on co-deposition process and coating surface morphology were investigated. The main conclusions were:
(1) High particle conductivity contributed to the co-deposition of particles, about 9.76wt% silicon content of coatings can be obtained for the 30%Si-Fe powder with the particle concentration of 50g/L, whereas that for Si powder was only 4.48wt%.
(2) The co-deposition of conductive Si-Fe powders into composite coatings in the mode of "cladding", while that for non-conductive Si powder was an "embedding" mode.
The authors gratefully acknowledged the financial support of National Natural Science Foundation of China(No.51664009), the Guizhou Provincial Natural Science Foundation of China(7101; 2016-1067), the Guizhou Provincial Education Department innovation group project(2016-043), and the Guizhou institute of technology project(KJZX17-015; XJGC20161212).
1. B.H. Park, B.S. Kang, S.D. Bu, T.W. Noh, J. Lee and W. Jo, Nature, 401 (1999) 682. 2. G.J. Cai, C.S. Li, B. Cai and Q.W. Wang, J. Magn. Magn. Mater., 430 (2017) 70. 3. R. Li, Q. Shen , L.M. Zhang and T. Zhang, J. Magn. Magn. Mater., 281 (2004) 135. 4. M. Garibaldi, L. Ashcroft, M. Simonelli and R. Hague, Acta Mater., 110 (2016) 207.
5. T. Yamaji, M. Abe, Y. Takada, K. Okada and T. Hiratani, J. Magn.Magn. Mater., 133 (1994) 187. 6. Z.Y. Cai, L.X. Zhang and Y.G. Li, Hydrometallurgy of china, 24 (2005) 83.
7. H. Krawiec, V. Vignal, M. Latkiewicz and F. Herbst, Appl. Surf. Sci.,427 (2018)1124.
8. H. Matsushima, Y. Fukunaka, S. Kikuchi, A. Ispas, A. Bund, Int. J. Electrochem. Sci., 7 (2012) 9345.
9. M. Alizadeh, H. Safaei, Appl. Surf. Sci., 456(2018) 195.
10.A.Laszczyńska, J.Winiarski, B.Szczygieł and I.Szczygieł, Appl. Surf. Sci., 369 (2016) 224 11.Y. Liang, Z.C. Guan, H.P. Wang, R.G. Du, Electrochem. Commun., 77 (2017) 120
12.N.P. Wasekar, S.M. Latha, M. Ramakrishna, D.S. Rao and G. Sundararajan, Mater. Design, 112 (2016) 140.
13.B. Bostani, N.P. Ahmad, S. Yazdani and R. Arghavanian, T. Nonferr. Metal. Soc., 28 (2018) 66. 14.H.J. Cho, J. Tam, M. Kovylina, Y.J. Kim and U. Erb, J. Alloy. Compd., 687 (2016) 570.
15.X.S. Su, Q.Q. Sun, J.J. Bai, Z.L. Wang and C. Zhao, Electrochim. Acta, 260 (2018) 477. 16.Y.J. Pan, H. Zhang and X.J. Wu, Electroplat & Finishing (Chinese), 26 (2004) 13.
17.Q. Long , Y.B. Zhong, T.X. Zheng and C.M. Liu, Chem. Res. Chinese. U., 30 (2014) 811. 18.M. Alizadeh and S. Narouei, J. Alloy. Compd., 772 (2019) 565.
19.M.K. Das, R.X. Li, J.Q. Qin, X.Y. Zhang, K. Das, A. Thueploy, S. Limpanart, Y. Boonyongmaneerat, M. Ma and R.P. Liu, Surf. Coat. Tech.,309 (2017) 337. 20.N. Gugliekmi, J. Electrochem. Soc.,1 19 (1972) 1009.
21.J.P. Celis，J.R. Roos and C. Buelens, J. Electrochem. Soc., 134 (1987) 1402. 22.J.P. Celis and J.R. Roos, J. Electrochem. Soc., 124 (1977) 1508.
23.Y. Suzuki and O. Asai,J. Electrochem. Soc., 134 (1987) 1905.
24.Q. Long, Y.B. Zhong, F. Li, H. Wang, J.F. Zhou, W.L. Ren and Z.S. Lei, J. Cent. South. Univ., 45 (2014) 367.
25.Q. Long, Y.B. Zhong, F. Li, C.M. Liu, J.F. Zhou, L.J. Fan and M.J. Li, Acta Metal. Sin., 49 (2013) 1201.
26.Q. Long, Y.B. Zhong, H. Wang, T.X. Zheng, J.F. Zhou and Z.M. Ren, Int. J. Min. Met. Mater., 21 (2014) 1175.
27.H. Matsushima, T. Nohira, I. Mogi and Y. Ito, Surf. Coat. Tech., 179 (2004) 245.